Polyvinyl chloride (/ˌpɒlivaɪnəl ˈklɔːraɪd/; colloquial: polyvinyl, vinyl; abbreviated: PVC) is the world's third-most widely produced synthetic plastic polymer, after polyethylene and polypropylene. About 40 million tonnes are produced per year.
PVC comes in two basic forms: rigid (sometimes abbreviated as RPVC) and flexible. The rigid form of PVC is used in construction for pipe and in profile applications such as doors and windows. It is also used in making bottles, non-food packaging, and cards (such as bank or membership cards). It can be made softer and more flexible by the addition of plasticizers, the most widely used being phthalates. In this form, it is also used in plumbing, electrical cable insulation, imitation leather, flooring, signage, phonograph records, inflatable products, and many applications where it replaces rubber. With cotton or linen, it is used to make canvas.
Pure polyvinyl chloride is a white, brittle solid. It is insoluble in alcohol but slightly soluble in tetrahydrofuran.
|−10.71×10−6 (SI, 22 °C) |
Except where otherwise noted, data are given for materials in their standard state (at 25 °C [77 °F], 100 kPa).
|Elongation at break||20–40%|
|Notch test||2–5 kJ/m2|
|Glass Transition Temperature||82 °C (180 °F)|
|Melting point||100 °C (212 °F) to 260 °C (500 °F)|
|Effective heat of combustion||17.95 MJ/kg|
|Specific heat (c)||0.9 kJ/(kg·K)|
|Water absorption (ASTM)||0.04–0.4|
|Dielectric Breakdown Voltage||40 MV/m|
PVC was accidentally synthesized in 1872 by German chemist Eugen Baumann. The polymer appeared as a white solid inside a flask of vinyl chloride that had been left exposed to sunlight. In the early 20th century the Russian chemist Ivan Ostromislensky and Fritz Klatte of the German chemical company Griesheim-Elektron both attempted to use PVC in commercial products, but difficulties in processing the rigid, sometimes brittle polymer thwarted their efforts. Waldo Semon and the B.F. Goodrich Company developed a method in 1926 to plasticize PVC by blending it with various additives. The result was a more flexible and more easily processed material that soon achieved widespread commercial use.
About 80% of production involves suspension polymerization. Emulsion polymerization accounts for about 12%, and bulk polymerization accounts for 8%. Suspension polymerization affords particles with average diameters of 100–180 μm, whereas emulsion polymerization gives much smaller particles of average size around 0.2 μm. VCM and water are introduced into the reactor along with a polymerization initiator and other additives. The contents of the reaction vessel are pressurized and continually mixed to maintain the suspension and ensure a uniform particle size of the PVC resin. The reaction is exothermic and thus requires cooling. As the volume is reduced during the reaction (PVC is denser than VCM), water is continually added to the mixture to maintain the suspension.
The polymerization of VCM is started by compounds called initiators that are mixed into the droplets. These compounds break down to start the radical chain reaction. Typical initiators include dioctanoyl peroxide and dicetyl peroxydicarbonate, both of which have fragile O-O bonds. Some initiators start the reaction rapidly but decay quickly, and other initiators have the opposite effect. A combination of two different initiators is often used to give a uniform rate of polymerization. After the polymer has grown by about 10 times, the short polymer precipitates inside the droplet of VCM, and polymerization continues with the precipitated, solvent-swollen particles. The weight average molecular weights of commercial polymers range from 100,000 to 200,000, and the number average molecular weights range from 45,000 to 64,000.
Once the reaction has run its course, the resulting PVC slurry is degassed and stripped to remove excess VCM, which is recycled. The polymer is then passed through a centrifuge to remove water. The slurry is further dried in a hot air bed, and the resulting powder is sieved before storage or pelletization. Normally, the resulting PVC has a VCM content of less than 1 part per million. Other production processes, such as micro-suspension polymerization and emulsion polymerization, produce PVC with smaller particle sizes (10 μm vs. 120–150 μm for suspension PVC) with slightly different properties and with somewhat different sets of applications.
PVC may be manufactured from either naphtha or ethylene feedstock. However in China, where there are substantial stocks, coal is the main starting material for the Calcium carbide process. The acetylene so generated is then converted to VCM which usually involves the use of a Mercury based catalyst. The process is also very energy intensive with much waste generated.
The polymers are linear and are strong. The monomers are mainly arranged head-to-tail, meaning that there are chlorides on alternating carbon centres. PVC has mainly an atactic stereochemistry, which means that the relative stereochemistry of the chloride centres are random. Some degree of syndiotacticity of the chain gives a few percent crystallinity that is influential on the properties of the material. About 57% of the mass of PVC is chlorine. The presence of chloride groups gives the polymer very different properties from the structurally related material polyethylene. The density is also higher than these structurally related plastics.
About half of the world's PVC production capacity is in China despite the closure of many Chinese PVC plants due to issues complying with environmental regulations and poor capacities of scale. The largest single producer of PVC as of 2018 is Shin-Etsu Chemical of Japan, with a global share of around 30%. The other major suppliers are based in North America and Western Europe.
The product of the polymerization process is unmodified PVC. Before PVC can be made into finished products, it always requires conversion into a compound by the incorporation of additives (but not necessarily all of the following) such as heat stabilizers, UV stabilizers, plasticizers, processing aids, impact modifiers, thermal modifiers, fillers, flame retardants, biocides, blowing agents and smoke suppressors, and, optionally, pigments. The choice of additives used for the PVC finished product is controlled by the cost performance requirements of the end use specification (underground pipe, window frames, intravenous tubing and flooring all have very different ingredients to suit their performance requirements). Previously, polychlorinated biphenyls (PCBs) were added to certain PVC products as flame retardants and stabilizers.
Most vinyl products contain plasticizers which dramatically improve their performance characteristic. The most common plasticizers are derivatives of phthalic acid. The materials are selected on their compatibility with the polymer, low volatility levels, and cost. These materials are usually oily colourless substances that mix well with the PVC particles. About 90% of the plasticizer market, estimated to be millions of tons per year worldwide, is dedicated to PVC.
While Di-2ethylhexylphthalate (DEHP) has been medically approved for many years for use in medical devices, it was permanently banned for use in children's products the US in 2008 by US Congress ; the PVC-DEHP combination had proved to be very suitable for making blood bags because DEHP stabilises red blood cells, minimising haemolysis (red blood cell rupture). However, DEHP is coming under increasing pressure in Europe. The assessment of potential risks related to phthalates, and in particular the use of DEHP in PVC medical devices, was subject to scientific and policy review by the European Union authorities, and on 21 March 2010, a specific labeling requirement was introduced across the EU for all devices containing phthalates that are classified as CMR (carcinogenic, mutagenic or toxic to reproduction). The label aims to enable healthcare professionals to use this equipment safely, and, where needed, take appropriate precautionary measures for patients at risk of over-exposure.
DEHP alternatives, which are gradually replacing it, are Adipates, Butyryltrihexylcitrate (BTHC), Cyclohexane-1,2-dicarboxylic acid, diisononylester (DINCH), Di(2-ethylhexyl)terephthalate, polymerics and trimellitic acid, 2-ethylhexylester (TOTM).
Liquid mixed metal stabilisers are used in several PVC flexible applications such as calendered films, extruded profiles, injection moulded soles and footwear, extruded hoses and plastisols where PVC paste is spread on to a backing (flooring, wall covering, artificial leather). Liquid mixed metal stabiliser systems are primarily based on barium, zinc and calcium carboxylates. In general liquid mixed metals like BaZn, CaZn require the addition of co-stabilisers, antioxidants and organo-phosphites to provide optimum performance.
BaZn stabilisers have successfully replaced cadmium-based stabilisers in Europe in many PVC semi-rigid and flexible applications.
In Europe, particularly Belgium, there has been a commitment to eliminate the use of cadmium (previously used as a part component of heat stabilizers in window profiles) and phase out lead-based heat stabilizers (as used in pipe and profile areas) such as liquid autodiachromate and calcium polyhydrocummate by 2015. According to the final report of Vinyl 2010 cadmium was eliminated across Europe by 2007. The progressive substitution of lead-based stabilizers is also confirmed in the same document showing a reduction of 75% since 2000 and ongoing. This is confirmed by the corresponding growth in calcium-based stabilizers, used as an alternative to lead-based stabilizers, more and more, also outside Europe.
Tin-based stabilizers are mainly used in Europe for rigid, transparent applications due to the high temperature processing conditions used. The situation in North America is different where tin systems are used for almost all rigid PVC applications. Tin stabilizers can be divided into two main groups, the first group containing those with tin-oxygen bonds and the second group with tin-sulphur bonds.
One of the most crucial additives are heat stabilizers. These agents minimize loss of HCl, a degradation process that starts above 70 °C. Once dehydrochlorination starts, it is autocatalytic. Many diverse agents have been used including, traditionally, derivatives of heavy metals (lead, cadmium). Increasingly, metallic soaps (metal "salts" of fatty acids) are favored, species such as calcium stearate. Addition levels vary typically from 2% to 4%. The choice of the best heat stabilizer depends on its cost effectiveness in the end use application, performance specification requirements, processing technology and regulatory approvals.
PVC is a thermoplastic polymer. Its properties are usually categorized based on rigid and flexible PVCs.
|Property||Rigid PVC||Flexible PVC|
|Thermal conductivity [W/(m·K)]||0.14–0.28||0.14–0.17|
|Yield strength||4,500–8,700 psi (31–60 MPa)||1,450–3,600 psi (10.0–24.8 MPa)|
|Young's modulus||490,000 psi (3.4 GPa)|
|Flexural strength (yield)||10,500 psi (72 MPa)|
|Compression strength [psi]||9,500 psi (66 MPa)|
|Coefficient of thermal expansion (linear) [mm/(mm °C)]||5×10−5|
|Vicat B [°C]||65–100||Not recommended|
|Resistivity [Ω m]||1016||1012–1015|
|Surface resistivity [Ω]||1013–1014||1011–1012|
PVC has high hardness and mechanical properties. The mechanical properties enhance with the molecular weight increasing but decrease with the temperature increasing. The mechanical properties of rigid PVC (uPVC) are very good; the elastic modulus can reach 1500-3,000 MPa. The soft PVC (flexible PVC) elastic limit is 1.5–15 MPa.
The heat stability of raw PVC is very poor, so the addition of a heat stabilizer during the process is necessary in order to ensure the product's properties. Traditional product PVC has a maximum operating temperature around 140°F (60°C) when heat distortion begins to occur. Melting temperatures range from 212°F to 500°F (100°C to 260°C) depending upon manufacture additives to the PVC. The linear expansion coefficient of rigid PVC is small and has good flame retardancy, the limiting oxygen index (LOI) being up to 45 or more. The LOI is the minimum concentration of oxygen, expressed as a percentage, that will support combustion of a polymer and noting that air has 20% content of oxygen.
As a thermoplastic, PVC has an inherent insulation that aids in reducing condensation formation and resisting internal temperature changes for hot and cold liquids.
Since the dielectric constant, dielectric loss tangent value, and volume resistivity are high, the corona resistance is not very good, and it is generally suitable for medium or low voltage and low frequency insulation materials.
PVC is chemically resistant to acids, salts, bases, fats, and alcohols, making it resistant to the corrosive effects of sewage, which is why it is so extensively utilized in sewer piping systems. It is also resistant to some solvents, this, however, is reserved mainly for uPVC (unplasticized PVC). Plasticized PVC, also known as PVC-P, is in some cases less resistant to solvents. For example, PVC is resistant to fuel and some paint thinners. Some solvents may only swell it or deform it but not dissolve it, but some, like tetrahydrofuran or acetone, may damage it.
Roughly half of the world's polyvinyl chloride resin manufactured annually is used for producing pipes for municipal and industrial applications. In the water distribution market, it accounts for 66% of the market in the U.S., and in sanitary sewer pipe applications, it accounts for 75%. Buried PVC pipes in both water and sanitary sewer applications that are 4 inches (100 mm) in diameter and larger are typically joined by means of a gasket-sealed joint. The most common type of gasket utilized in North America is a metal reinforced elastomer, commonly referred to as a Rieber sealing system. Its light weight, low cost, and low maintenance make it attractive. However, it must be carefully installed and bedded to ensure longitudinal cracking and overbelling does not occur. Additionally, PVC pipes can be fused together using various solvent cements, or heat-fused (butt-fusion process, similar to joining high-density polyethylene (HDPE) pipe), creating permanent joints that are virtually impervious to leakage.
In February 2007 the California Building Standards Code was updated to approve the use of chlorinated polyvinyl chloride (CPVC) pipe for use in residential water supply piping systems. CPVC has been a nationally accepted material in the U.S. since 1982; California, however, has permitted only limited use since 2001. The Department of Housing and Community Development prepared and certified an environmental impact statement resulting in a recommendation that the commission adopt and approve the use of CPVC. The commission's vote was unanimous, and CPVC has been placed in the 2007 California Plumbing Code.
PVC is commonly used as the insulation on electrical cables such as teck; PVC used for this purpose needs to be plasticized. Flexible PVC coated wire and cable for electrical use has traditionally been stabilised with lead, but these are being replaced with calcium-based systems.
In a fire, PVC-coated wires can form hydrogen chloride fumes; the chlorine serves to scavenge free radicals and is the source of the material's fire retardance. While hydrogen chloride fumes can also pose a health hazard in their own right, it dissolves in moisture and breaks down onto surfaces, particularly in areas where the air is cool enough to breathe, and is not available for inhalation. Frequently in applications where smoke is a major hazard (notably in tunnels and communal areas), PVC-free cable insulation is preferred, such as low smoke zero halogen (LSZH) insulation.
PVC is a common, strong but lightweight plastic used in construction. It is made softer and more flexible by the addition of plasticizers. If no plasticizers are added, it is known as uPVC (unplasticized polyvinyl chloride) or rigid PVC.
uPVC is extensively used in the building industry as a low-maintenance material, particularly in Ireland, the United Kingdom, in the United States and Canada. In the U.S. and Canada it is known as vinyl or vinyl siding. The material comes in a range of colors and finishes, including a photo-effect wood finish, and is used as a substitute for painted wood, mostly for window frames and sills when installing insulated glazing in new buildings; or to replace older single-glazed windows, as it does not decompose and is weather-resistant. Other uses include fascia, and siding or weatherboarding. This material has almost entirely replaced the use of cast iron for plumbing and drainage, being used for waste pipes, drainpipes, gutters and downspouts. uPVC is known as having strong resistance against chemicals, sunlight, and oxidation from water.
Polyvinyl chloride is formed in flat sheets in a variety of thicknesses and colors. As flat sheets, PVC is often expanded to create voids in the interior of the material, providing additional thickness without additional weight and minimal extra cost (see Closed-cell PVC foamboard). Sheets are cut using saws and rotary cutting equipment. Plasticized PVC is also used to produce thin, colored, or clear, adhesive-backed films referred to simply as vinyl. These films are typically cut on a computer-controlled plotter (see Vinyl cutter) or printed in a wide-format printer. These sheets and films are used to produce a wide variety of commercial signage products, including car body stripes and stickers.
PVC fabric has a niche role in specialty clothing, to either create a artificial leather material or at times simply for its effect. PVC clothing is common in Goth, Punk, clothing fetish and alternative fashions. PVC is less expensive than rubber, leather, and latex which it is used to simulate.
The two main application areas for single-use medically approved PVC compounds are flexible containers and tubing: containers used for blood and blood components, for urine collection or for ostomy products and tubing used for blood taking and blood giving sets, catheters, heart-lung bypass sets, hemodialysis sets etc. In Europe the consumption of PVC for medical devices is approximately 85,000 tons each year. Almost one third of plastic-based medical devices are made from PVC. The reasons for using flexible PVC in these applications for over 50 years are numerous and based on cost effectiveness linked to transparency, light weight, softness, tear strength, kink resistance, suitability for sterilization and biocompatibility.
Flexible PVC flooring is inexpensive and used in a variety of buildings, including homes, hospitals, offices, and schools. Complex and 3D designs are possible, which are then protected by a clear wear layer. A middle vinyl foam layer also gives a comfortable and safe feel. The smooth, tough surface of the upper wear layer prevents the buildup of dirt, which prevents microbes from breeding in areas that need to be kept sterile, such as hospitals and clinics.
PVC may be extruded under pressure to encase wire rope and aircraft cable used for general purpose applications. PVC coated wire rope is easier to handle, resists corrosion and abrasion, and may be color-coded for increased visibility. It is found in a variety of industries and environments both indoor and out.
PVC has been used for a host of consumer products. One of its earliest mass-market consumer applications was vinyl record production. More recent examples include wallcovering, greenhouses, home playgrounds, foam and other toys, custom truck toppers (tarpaulins), ceiling tiles and other kinds of interior cladding.
PVC piping is cheaper than metals used in musical instrument making; it is therefore a common alternative when making instruments, often for leisure or for rarer instruments such as the contrabass flute.
PVC can be usefully modified by chlorination, which increases its chlorine content to or above 67%. Chlorinated polyvinyl chloride, (CPVC), as it is called, is produced by chlorination of aqueous solution of suspension PVC particles followed by exposure to UV light which initiates the free-radical chlorination. The reaction produces CPVC, which has thermal and chemical properties that are superior to PVC.
Degradation during service life, or after careless disposal, is a chemical change that drastically reduces the average molecular weight of the polyvinyl chloride polymer. Since the mechanical integrity of a plastic depends on its high average molecular weight, wear and tear inevitably weakens the material. Weathering degradation of plastics results in their surface embrittlement and microcracking, yielding microparticles that continue on in the environment. Also known as microplastics, these particles act like sponges and soak up persistent organic pollutants (POPs) around them. Thus laden with high levels of POPs, the microparticles are often ingested by organisms in the biosphere.
However, there is evidence that three of the polymers (HDPE, LDPE, and PP) consistently soaked up POPs at concentrations an order of magnitude higher than did the remaining two (PVC and PET). After 12 months of exposure, for example, there was a 34-fold difference in average total POPs amassed on LDPE compared to PET at one location. At another site, average total POPs adhered to HDPE was nearly 30 times that of PVC. The researchers think that differences in the size and shape of the polymer molecules can explain why some accumulate more pollutants than others. The fungus Aspergillus fumigatus effectively degrades plasticized PVC. Phanerochaete chrysosporium was grown on PVC in a mineral salt agar. Phanerochaete chrysosporium, Lentinus tigrinus, Aspergillus niger, and Aspergillus sydowii can effectively degrade PVC.
Phthalates, which are incorporated into plastics as plasticizers, comprise approximately 70% of the U.S. plasticizer market; phthalates are by design not covalently bound to the polymer matrix, which makes them highly susceptible to leaching. Phthalates are contained in plastics at high percentages. For example, they can contribute up to 40% by weight to intravenous medical bags and up to 80% by weight in medical tubing. Vinyl products are pervasive—including toys, car interiors, shower curtains, and flooring—and initially release chemical gases into the air. Some studies indicate that this outgassing of additives may contribute to health complications, and have resulted in a call for banning the use of DEHP on shower curtains, among other uses. Japanese car companies Toyota, Nissan, and Honda eliminated the use of PVC in car interiors since 2007.
In 2004 a joint Swedish-Danish research team found a statistical association between allergies in children and indoor air levels of DEHP and BBzP (butyl benzyl phthalate), which is used in vinyl flooring. In December 2006, the European Chemicals Bureau of the European Commission released a final draft risk assessment of BBzP which found "no concern" for consumer exposure including exposure to children.
Risk assessments have led to the classification of low molecular weight and labeling as Category 1B Reproductive agents. Three of these phthalates, DBP, BBP and DEHP were included on annex XIV of the REACH regulation in February 2011 and will be phased out by the EU by February 2015 unless an application for authorisation is made before July 2013 and an authorisation granted. DIBP is still on the REACH Candidate List for Authorisation. Environmental Science & Technology, a peer reviewed journal published by the American Chemical Society states that it is completely safe.
In 2008 the European Union's Scientific Committee on Emerging and Newly Identified Health Risks (SCENIHR) reviewed the safety of DEHP in medical devices. The SCENIHR report states that certain medical procedures used in high risk patients result in a significant exposure to DEHP and concludes there is still a reason for having some concerns about the exposure of prematurely born male babies to medical devices containing DEHP. The Committee said there are some alternative plasticizers available for which there is sufficient toxicological data to indicate a lower hazard compared to DEHP but added that the functionality of these plasticizers should be assessed before they can be used as an alternative for DEHP in PVC medical devices. Risk assessment results have shown positive results regarding the safe use of High Molecular Weight Phthalates. They have all been registered for REACH and do not require any classification for health and environmental effects, nor are they on the Candidate List for Authorisation. High phthalates are not CMR (carcinogenic, mutagenic or toxic for reproduction), neither are they considered endocrine disruptors.
In the EU Risk Assessment the European Commission has confirmed that Di-isononyl phthalate (DINP) and Di-isodecyl phthalate (DIDP) pose no risk to either human health or the environment from any current use. The European Commission's findings (published in the EU Official Journal on 13 April 2006) confirm the outcome of a risk assessment involving more than 10 years of extensive scientific evaluation by EU regulators. Following the recent adoption of EU legislation with the regard to the marketing and use of DINP in toys and childcare articles, the risk assessment conclusions clearly state that there is no need for any further measures to regulate the use of DINP. In Europe and in some other parts of the world, the use of DINP in toys and childcare items has been restricted as a precautionary measure. In Europe, for example, DINP can no longer be used in toys and childcare items that can be put in the mouth even though the EU scientific risk assessment concluded that its use in toys does not pose a risk to human health or the environment. The rigorous EU risk assessments, which include a high degree of conservatism and built-in safety factors, have been carried out under the strict supervision of the European Commission and provide a clear scientific evaluation on which to judge whether or not a particular substance can be safely used.
The FDA Paper titled "Safety Assessment of Di(2-ethylhexyl)phthalate (DEHP)Released from PVC Medical Devices" states that [220.127.116.11] Critically ill or injured patients may be at increased risk of developing adverse health effects from DEHP, not only by virtue of increased exposure relative to the general population, but also because of the physiological and pharmacodynamic changes that occur in these patients compared to healthy individuals.
In Europe (EU 28) the use of lead-based stabilizers was gradually replaced. The VinylPlus voluntary commitment which began in 2000, saw European Stabiliser Producers Association (ESPA) members complete the replacement of Pb-based stabilisers in 2015.
In the early 1970s, the carcinogenicity of vinyl chloride (usually called vinyl chloride monomer or VCM) was linked to cancers in workers in the polyvinyl chloride industry. Specifically workers in polymerization section of a B.F. Goodrich plant near Louisville, Kentucky, were diagnosed with liver angiosarcoma also known as hemangiosarcoma, a rare disease. Since that time, studies of PVC workers in Australia, Italy, Germany, and the UK have all associated certain types of occupational cancers with exposure to vinyl chloride, and it has become accepted that VCM is a carcinogen. Technology for removal of VCM from products has become stringent, commensurate with the associated regulations.
PVC produces HCl upon combustion almost quantitatively related to its chlorine content. Extensive studies in Europe indicate that the chlorine found in emitted dioxins is not derived from HCl in the flue gases. Instead, most dioxins arise in the condensed solid phase by the reaction of inorganic chlorides with graphitic structures in char-containing ash particles. Copper acts as a catalyst for these reactions.
Studies of household waste burning indicate consistent increases in dioxin generation with increasing PVC concentrations. According to the EPA dioxin inventory, landfill fires are likely to represent an even larger source of dioxin to the environment. A survey of international studies consistently identifies high dioxin concentrations in areas affected by open waste burning and a study that looked at the homologue pattern found the sample with the highest dioxin concentration was "typical for the pyrolysis of PVC". Other EU studies indicate that PVC likely "accounts for the overwhelming majority of chlorine that is available for dioxin formation during landfill fires."
The next largest sources of dioxin in the EPA inventory are medical and municipal waste incinerators. Various studies have been conducted that reach contradictory results. For instance a study of commercial-scale incinerators showed no relationship between the PVC content of the waste and dioxin emissions. Other studies have shown a clear correlation between dioxin formation and chloride content and indicate that PVC is a significant contributor to the formation of both dioxin and PCB in incinerators.
In February 2007, the Technical and Scientific Advisory Committee of the US Green Building Council (USGBC) released its report on a PVC avoidance related materials credit for the LEED Green Building Rating system. The report concludes that "no single material shows up as the best across all the human health and environmental impact categories, nor as the worst" but that the "risk of dioxin emissions puts PVC consistently among the worst materials for human health impacts."
In Europe the overwhelming importance of combustion conditions on dioxin formation has been established by numerous researchers. The single most important factor in forming dioxin-like compounds is the temperature of the combustion gases. Oxygen concentration also plays a major role on dioxin formation, but not the chlorine content.
The design of modern incinerators minimises PCDD/F formation by optimising the stability of the thermal process. To comply with the EU emission limit of 0.1 ng I-TEQ/m3 modern incinerators operate in conditions minimising dioxin formation and are equipped with pollution control devices which catch the low amounts produced. Recent information is showing for example that dioxin levels in populations near incinerators in Lisbon and Madeira have not risen since the plants began operating in 1999 and 2002 respectively.
Several studies have also shown that removing PVC from waste would not significantly reduce the quantity of dioxins emitted. The European Union Commission published in July 2000 a Green Paper on the Environmental Issues of PVC. " The Commission states (page 27) that it has been suggested that the reduction of the chlorine content in the waste can contribute to the reduction of dioxin formation, even though the actual mechanism is not fully understood. The influence on the reduction is also expected to be a second or third order relationship. It is most likely that the main incineration parameters, such as the temperature and the oxygen concentration, have a major influence on the dioxin formation". The Green Paper states further that at the current levels of chlorine in municipal waste, there does not seem to be a direct quantitative relationship between chlorine content and dioxin formation.
A study commissioned by the European Commission on "Life Cycle Assessment of PVC and of principal competing materials" states that "Recent studies show that the presence of PVC has no significant effect on the amount of dioxins released through incineration of plastic waste."
The European waste hierarchy refers to the five steps included in the article 4 of the Waste Framework Directive:
The European Commission has set new rules to promote the recovery of PVC waste for use in a number of construction products. It says: "The use of recovered PVC should be encouraged in the manufacture of certain construction products because it allows the reuse of old PVC ... This avoids PVC being discarded in landfills or incinerated causing release of carbon dioxide and cadmium in the environment".
In Europe, developments in PVC waste management have been monitored by Vinyl 2010, established in 2000. Vinyl 2010's objective was to recycle 200,000 tonnes of post-consumer PVC waste per year in Europe by the end of 2010, excluding waste streams already subject to other or more specific legislation (such as the European Directives on End-of-Life Vehicles, Packaging and Waste Electric and Electronic Equipment).
Since June 2011, it is followed by VinylPlus, a new set of targets for sustainable development. Its main target is to recycle 800,000 tonnes/year of PVC by 2020 including 100,000 tonnes of difficult to recycle waste. One facilitator for collection and recycling of PVC waste is Recovinyl. The reported and audited recycled PVC tonnage in 2016 was 568,695 tonnes.
One approach to address the problem of waste PVC is also through the process called Vinyloop. It is a mechanical recycling process using a solvent to separate PVC from other materials. This solvent turns in a closed loop process in which the solvent is recycled. Recycled PVC is used in place of virgin PVC in various applications: coatings for swimming pools, shoe soles, hoses, diaphragms tunnel, coated fabrics, PVC sheets. This recycled PVC's primary energy demand is 46 percent lower than conventional produced PVC. So the use of recycled material leads to a significant better ecological footprint. The global warming potential is 39 percent lower.
In January 2012 a major U.S. West Coast healthcare provider, Kaiser Permanente, announced that it will no longer buy intravenous (IV) medical equipment made with polyvinyl chloride (PVC) and DEHP (di-2-ethyl hexyl phthalate) type plasticizers.
Plasticized PVC is a common material for medical gloves. Due to vinyl gloves having less flexibility and elasticity, several guidelines recommend either latex or nitrile gloves for clinical care and procedures that require manual dexterity and/or that involve patient contact for more than a brief period. Vinyl gloves show poor resistance to many chemicals, including glutaraldehyde-based products and alcohols used in formulation of disinfectants for swabbing down work surfaces or in hand rubs. The additives in PVC are also known to cause skin reactions such as allergic contact dermatitis. These are for example the antioxidant bisphenol A, the biocide benzisothiazolinone, propylene glycol/adipate polyester and ethylhexylmaleate.
PVC is made from petroleum. The production process also uses sodium chloride. Recycled PVC is broken down into small chips, impurities removed, and the product refined to make pure white PVC. It can be recycled roughly seven times and has a lifespan of around 140 years.
In the UK, approximately 400 tonnes of PVC are recycled every month. Property owners can recycle it through nationwide collection depots. The Olympic Delivery Authority (ODA), for example, after initially rejecting PVC as material for different temporary venues of the London Olympics 2012, has reviewed its decision and developed a policy for its use. This policy highlighted that the functional properties of PVC make it the most appropriate material in certain circumstances while taking into consideration the environmental and social impacts across the whole life cycle, e.g. the rate for recycling or reuse and the percentage of recycled content. Temporary parts, like roofing covers of the Olympic Stadium, the Water Polo Arena, and the Royal Artillery Barracks, would be deconstructed and a part recycled in the VinyLoop process.
Acroosteolysis is resorption of the distal bony phalanges. Acroosteolysis has two patterns of resorption in adults: diffuse and bandlike.
The diffuse pattern of resorption has a widely diverse differential diagnosis which includes: pyknodysostosis, collagen vascular disease and vasculitis, Raynaud's neuropathy, trauma, epidermolysis bullosa, psoriasis, frostbite, sarcoidosis, hypertrophic osteoarthropathy, acromegaly, and advanced leprosy.The bandlike pattern of resorption may be seen with polyvinyl chloride exposure and Hadju-Cheney syndrome.A mnemonic commonly used for acro-osteolysis is PINCHFO.Pyknodysostosis, Psoriasis,
Injury (thermal burn, frostbite),
Collagen vascular disease (scleroderma, Raynaud's),
Familial (Hadju-Cheney, progeria),
Occupational (polyvinyl exposure),
Acroosteolysis may be associated with minimal skin changes or with ischemic skin lesions that may result in digital necrosis.Angiosarcoma
Angiosarcoma is a cancer of the cells that line the walls of blood vessels or lymphatic vessels. The lining of the vessel walls is called the endothelium. However, they should not be confused with cherry hemangiomas.
Most tumors of visceral blood and lymphatic vessel walls are cancerous (malignant). Because these cancers are carried by the blood flow or lymphatic flow, they can more easily metastasize to distant sites, particularly the liver and lungs.
Angiosarcomas show signs of hemorrhage and necrosis. Pathologically, tumor cells show increased nuclear to cytoplasm ratio, nuclear hyperchromasia, nuclear pleomorphism and high mitotic activity.In dogs, hemangiosarcoma is relatively common, especially in larger breeds such as golden retrievers and Labrador retrievers. In humans, hemangiosarcomas and lymphangiosarcomas of the skin are uncommon. Angiosarcoma of the liver, a rare fatal tumor, has been seen in workers intensively exposed to the gas vinyl chloride monomer (VCM) for prolonged periods while working in polyvinyl chloride (PVC) polymerization plants. It has also been associated with individuals exposed to arsenic-containing insecticides and Thorotrast.Chlorinated polyvinyl chloride
Chlorinated polyvinyl chloride (CPVC) is a thermoplastic produced by chlorination of polyvinyl chloride (PVC) resin, which is significantly more flexible and can withstand higher temperatures than standard PVC. Uses include hot and cold water delivery pipes and industrial liquid handling. CPVC, as PVC, is deemed safe for the transport and use of potable water, potable meaning water used for drinking, cooking, and bathing.Commodity plastics
Commodity plastics are plastics that are used in high volume and wide range of applications, such as film for packaging, photographic and magnetic tape, clothing, beverage and trash containers and a variety of household products where mechanical properties and service environments are not critical. Such plastics exhibit relatively low mechanical properties and are of low cost. The range of products includes Plates, Cups, Carrying Trays, Medical Trays, Containers, Seeding Trays, Printed Material and other disposable items.Examples of commodity plastics are polyethylene, polypropylene, polystyrene, polyvinyl chloride, poly(methyl methacrylate) and more.Hanwha Chemical
Hanwha Chemical Co, Ltd. (Hangul: 한화케미칼) is a South Korean chemical company headquartered in Seoul and an affiliate of the Hanwha Group.
Established in 1965, Hanwha Chemical has been at the forefront of the advancement of Korea’s chemical industry. Starting with Korea’s first production of PVC (Polyvinyl Chloride), Hanwha Chemical has been producing a full array of basic petrochemical products including LDPE (Low Density Polyethylene), LLDPE (Linear Low Density Polyethylene), and CA (Chlor-Alkali), all of which serve as the foundation for an extensive range of industries. Hanwha Chemical’s products exist in people’s daily lives in various forms and contribute to improving the overall quality of life.
Hanwha Chemical is also expanding its assets to include Polysilicon, a core feedstock for solar cells as well as specialty products like CPVC (Chlorinated Polyvinyl Chloride) and hydrogenated resins.IPK Acrylic-polyvinyl chloride
IPK Acrylic-polyvinyl chloride (IPK, IPK Acrylic PVC, IPK Thermoformable Sheet, IPK Kydex) is a line of thermoplastic acrylic-polyvinyl chloride composite material. It has a chemical structure similar to Kydex with an Acrylic-polyvinyl chloride substrate and white cap for screen printing onto the material.
Kydex sheet was originally produced in 1965 by Rohm and Haas, having been designed for use in aircraft interiors. In recent years, Kydex has gained a hobbyist following for a wide variety of applications, including firearm holsters and sheaths for knives.IPK Acrylic-polyvinyl chloride was developed by Interstate Plastics in 2012 and sold under the registered trademark IPK. Interstate Plastics claims the material offers an alternative to thermoformable plastic sheets while providing a printable surface for custom designs and patterns. Most vinyl sign print shops are able to print custom designs or patterns onto the material. IPK is currently the only thermoforming sheet on the market sold with a printable cap.Kydex
KYDEX(r) is a line of thermoplastic acrylic-polyvinyl chloride materials manufactured by Sekisui SPI. It has a wide variety of applications, including for aircraft bulkheads, firearm holsters, sheaths, and for knives.
Similar acrylic polyvinyl chloride material (IPK Acrylic-polyvinyl chloride) is manufactured by Emco Plastics and Interstate Plastics, which carries nearly identical properties with an added layer for screen printing.Naugahyde
Naugahyde is an American brand of artificial leather. Naugahyde is a composite knit fabric backing and expanded polyvinyl chloride (PVC) plastic coating. It was developed by Byron A. Hunter, senior chemist at the United States Rubber Company, and is now manufactured and sold by Uniroyal Engineered Products, LLC, a publicly held company under Invisa, Inc. Invisa also owns Wardle Storeys in the UK.
Its name, first used as a trademark in 1936, comes from the name of Naugatuck, Connecticut, where it was first produced. It is now manufactured in Stoughton, Wisconsin.Petkim
Petkim Petrokimya Holding A.Ş. is the leading petrochemical company of Turkey. Founded on April 3, 1965, the main plant complex is located in Yarımca, Izmit. From 1985 on a second complex has been constructed in Aliağa, İzmir.Specializing in petrochemical manufacturing, the company produces ethylene, polyethylene, polyvinyl chloride, polypropylene and other chemical building blocks for use in the manufacture of plastics, textiles, and other consumer and industrial products. The company has 14 manufacturing plants supplying a significant portion of petrochemicals used in Turkey. The company also exports products to the United States, and countries in Europe, the Middle East, Africa, and Asia.Petkim is listed on the Istanbul Stock Exchange.
Petlim is a container port currently being built near the town of Aliağa.Plastic pipework
Plastic pipe is a tubular section, or hollow cylinder, made of plastic. It is usually, but not necessarily, of circular cross-section, used mainly to convey substances which can flow—liquids and gases (fluids), slurries, powders and masses of small solids. It can also be used for structural applications; hollow pipes are far stiffer per unit weight than solid members.
Plastic pipework is used for the conveyance of drinking water, waste water, chemicals, heating fluid and cooling fluids, foodstuffs, ultra-pure liquids, slurries, gases, compressed air and vacuum system applications.Pocket protector
A pocket protector is a sheath designed to hold writing instruments and other small implements, such as slide rules, while preventing them from damaging the wearer's shirt pocket (e.g., by tearing or staining by a leaky pen). The pocket protector is designed to fit neatly inside the breast pocket of a shirt, and may accommodate pens, pencils, screwdrivers, small slide rules, and various other small items. A flap overlapping the pocket exterior helps to secure the pocket protector in place.
The pocket protector was invented during World War II by Hurley Smith while he was working in Buffalo, New York. He was awarded ‹See Tfd›US 2417786 for the device on March 18, 1947; the patent was filed on June 3, 1943.A competing claim for the invention came from Long Island plastics magnate Gerson Strassberg around 1952. Strassberg was working on plastic sleeves for bankbooks. One day he placed one that he was working on into his shirt pocket while he took a phone call. When he noticed it there, he realized it would make a great product.Originally fashioned from polyvinyl chloride (PVC), pocket protectors were first marketed toward corporations as branded promotional fare. However, a more general market for the product soon arose, made up of students, engineers (prominently mechanical), and white-collar workers in sundry fields. The accessory has become part of a "nerd" or "geek" fashion stereotype, probably because of its association with engineers or students.Polymeric foam
A polymeric foam is a foam, in liquid or solidified form, formed from polymers.
Ethylene-vinyl acetate (EVA) foam, the copolymers of ethylene and vinyl acetate; also referred to as polyethylene-vinyl acetate (PEVA)
Low-density polyethylene (LDPE) foam, first grade of polyethylene (PE)
Nitrile rubber (NBR) foam, the copolymers of acrylonitrile (ACN) and butadiene
Polychloroprene foam or Neoprene
Polypropylene (PP) foam, including expanded polypropylene (EPP) and polypropylene paper (PPP)
Polystyrene (PS) foam, including expanded polystyrene (EPS), extruded polystyrene foam (XPS) and sometimes polystyrene paper (PSP)
Styrofoam, including extruded polystyrene foam (XPS) and sometimes expanded polystyrene (EPS)
Polyurethane (PU) foam
LRPu low-resilience polyurethane
Polyethylene foam, as used in PEF rod
Polyvinyl chloride (PVC) foam
Closed-cell PVC foamboard
Microcellular foamPolyvinyl chloride acetate
Polyvinyl chloride acetate (PVCA) is a thermoplastic copolymer of vinyl chloride and vinyl acetate. It is used in the manufacture of electrical insulation, of protective coverings (including garments), and of credit cards and swipe cards.Thermoplastic
A thermoplastic, or thermosoftening plastic, is a plastic polymer material that becomes pliable or moldable at a certain elevated temperature and solidifies upon cooling.Most thermoplastics have a high molecular weight. The polymer chains associate by intermolecular forces, which weaken rapidly with increased temperature, yielding a viscous liquid. In this state, thermoplastics may be reshaped and are typically used to produce parts by various polymer processing techniques such as injection molding, compression molding, calendering, and extrusion. Thermoplastics differ from thermosetting polymers which form irreversible chemical bonds during the curing process. Thermosets do not melt when heated, but typically decompose and do not reform upon cooling.
Above its glass transition temperature and below its melting point, the physical properties of a thermoplastic change drastically without an associated phase change. Some thermoplastics do not fully crystallize below the glass transition temperature, retaining some or all of their amorphous characteristics. Amorphous and semi-amorphous plastics are used when high optical clarity is necessary, as light is scattered strongly by crystallites larger than its wavelength. Amorphous and semi-amorphous plastics are less resistant to chemical attack and environmental stress cracking because they lack a crystalline structure.
Brittleness can be decreased with the addition of plasticizers, which increases the mobility of amorphous chain segments to effectively lower the glass transition temperature. Modification of the polymer through copolymerization or through the addition of non-reactive side chains to monomers before polymerization can also lower it. Before these techniques were employed, plastic automobile parts would often crack when exposed to cold temperatures.These are linear or slightly branched long chain molecules capable of repeatedly softening on heating and hardening on cooling.Tracheal tube
A tracheal tube is a catheter that is inserted into the trachea for the primary purpose of establishing and maintaining a patent airway and to ensure the adequate exchange of oxygen and carbon dioxide.
Many different types of tracheal tubes are available, suited for different specific applications:
An endotracheal tube is a specific type of tracheal tube that is nearly always inserted through the mouth (orotracheal) or nose (nasotracheal).
A tracheostomy tube is another type of tracheal tube; this 2–3-inch-long (51–76 mm) curved metal or plastic tube may be inserted into a tracheostomy stoma (following a tracheotomy) to maintain a patent lumen.
A tracheal button is a rigid plastic cannula about 1 inch in length that can be placed into the tracheostomy after removal of a tracheostomy tube to maintain patency of the lumen.Vinyl
Vinyl may refer to:
Vinyl group, a class of organic molecules in chemistry
Polyvinyl chloride (PVC), a particular vinyl polymer
Vinyl composition tile, floortiles
Vinyl polymer, a group of polymers derived from vinyl monomers
Vinyl siding, an outer covering of a houseVinyl composition tile
Vinyl composition tile (VCT) is a finished flooring material used primarily in commercial and institutional applications. Modern vinyl floor tiles and sheet flooring and versions of those products sold since the early 1980s are composed of colored polyvinyl chloride (PVC) chips formed into solid sheets of varying thicknesses (1/8" is most common) by heat and pressure. Floor tiles are cut into modular shapes such 12" x 12" squares or 12" x 24" rectangles. In installation the floor tiles or sheet flooring are applied to a smooth, leveled sub-floor using a specially formulated vinyl adhesive or tile mastic that remains pliable. In commercial applications some tiles are typically waxed and buffed using special materials and equipment.
Modern vinyl floor tile is frequently chosen for high-traffic areas because of its low cost, durability, and ease of maintenance. Vinyl tiles have high resilience to abrasion and impact damage and can be repeatedly refinished with chemical strippers and mechanical buffing equipment. If properly installed, tiles can be easily removed and replaced when damaged. Tiles are available in a variety of colors from several major flooring manufacturers. Some manufacturers have created vinyl tiles that very closely resemble wood, stone, terrazzo, and concrete and hundreds of varying patterns.Vinyl polymer
Vinyl polymers are a group of polymers derived from vinyl monomers of the type CH2=CHR. Their backbone is an extended alkane chain ...-CH2-CHR-CH2-CHR-..). In popular usage, "vinyl" refers only to polyvinyl chloride (PVC).Vinyon
Vinyon is a synthetic fiber made from polyvinyl chloride. In some countries other than the United States, vinyon fibers are referred to as polyvinyl chloride fibers. It can bind non-woven fibers and fabrics. It was invented in 1939.
It has the same health problems associated with chlorinated polymers. In the past, Vinyon was used a substitute for plant-based filters in tea bags.
|Miscellaneous additives incl. PHCs|
|Environment and health|